Influence of Deposition Condition on Y 2 O 3 Coatings Produced by Pulsed Electrophoretic Deposition

Y 2 O 3 nanoparticle suspension aqueous solution was prepared using citric acid. Then, Y 2 O 3 film was deposited using this solution with pulsed electrophoretic deposition (EPD). A dense Y 2 O 3 film of 25.7 μm thickness was obtained with deposition conditions of 0.5 wt% Y 2 O 3 concentration, bias voltage of 0.5 V, and bias frequency of 1 kHz. The respective resistivities of the as-deposited film and films heat-treated at 200C and 400Cwere 2.84 × 10Ω⋅cm, 5.36 × 10Ω⋅cm, and 2.05 × 10Ω⋅cm. A 59.8 μm thick dense Y 2 O 3 film was obtained using two-step deposition with change of the bias voltage: a first step of 0.5 V and a second step of 2.0 V.


Introduction
Recently, semiconductor production equipment systems for dry etching have become widely used [1].Carbon fluoride gas plasma is commonly used for high-speed etching of silicon wafers [2].During production in equipment chambers, these plasmas invariably contact ceramic walls made of materials such as SiO 2 or Al 2 O 3 , thereby causing erosion of the equipment and producing contamination particles [3].High plasma resistance is therefore necessary for the etching chamber.As a new component of dry-etching equipment, Y 2 O 3 is an anticipated candidate because of its excellent resistance to plasma corrosion [4].
Substrate materials of semiconductor production equipment system components are commonly aluminum-based alloys or stainless steel.In fact, Y 2 O 3 coatings are applied onto these substrates [5] using coating methods that include CVD [6], plasma spray [7], and aerosol deposition [4].These coating techniques require vacuum systems, which are expensive resources that entail great difficulty for coating large substrates.However, the substrate materials described above show high electrical conductivity.Electrophoretic deposition (EPD), one candidate for use as Y 2 O 3 coating method, enables coatings to be obtained on both planar and complex shape substrates such as spheres and bending metal parts [8].Furthermore, films can be formed using "powders" alone.Therefore, its limitations are few for source materials.For those reasons, some EPD methods are quite suitable for Y 2 O 3 coating onto alloy components of semiconductor production equipment.
In this investigation, Y 2 O 3 coating was investigated using Y 2 O 3 suspension aqueous solution with a pulsed EPD method.The use of AC or pulsed bias induces very little decomposition of water.Therefore, gas bubble formation in the deposits is eliminated or is greatly minimized [9].Using a pulsed EPD method to form Y 2 O 3 coatings in this investigation, we observed the effects of deposition conditions on Y 2 O 3 film formation.

Experimental Procedure
As a starting material, Y 2 O 3 (Nanophase Technologies Corp., USA) powder was used.It had particle size of 20-90 nm.Y 2 O 3 powder was put into a 1.0 wt% citric acid (Wako Pure Chemical Inds.Ltd., Osaka, Japan) aqueous solution with the Y 2 O 3 weight ratio of 0.5-5 wt%.Citric acid was used to stabilize the Y 2 O 3 suspension aqueous solution [10].The resulting Y 2 O 3 suspension solution was subjected to ultrasonic waves.The suspension solution was stirred.Stainless steel was used as the substrate.It was soaked in the suspension.Y 2 O 3 deposition on this substrate was conducted by application of a pulsed bias to substrates using a universal source (HP-3245A; Agilent Technologies Inc.).The bias voltage applied to substrates was −0.5 to −5.0 V (hereinafter, we call a negative bias value simply an absolute bias value).The bias frequency was 10-100 kHz.Deposition was conducted for 1 h.The deposited films were dried at 70 ∘ C for 1 day.
The grain size and form of the Y 2 O 3 particles were evaluated using transmission electron microscopy (TEM, EM-002B; Topcon Corp.).The microstructures of the resulting powders were observed using a scanning electron microscope (SEM, JSM-6510; JEOL).Resistivity of the resulting films was evaluated along with the deposition direction using a twoprobe method with a DC source (HP-3654; Hewlett Packard Co.) and a digital voltmeter (HP34401; Hewlett Packard Co.).

Results and Discussion
The Y 2 O 3 particle microstructure was observed using TEM, as presented in Figure 1.The Y 2 O 3 particle grain size was 20-90 nm.The form was spheroidal.The Y 2 O 3 coatings were applied with different conditions of concentration (wt%) of suspension solution, frequency of applied bias voltage, and the applied bias voltage using Y 2 O 3 particles.The optimal concentration in this study was found to be 0.5 wt%.
To confirm the effects of bias frequency, Y 2 O 3 films were deposited to the substrates with different bias frequencies.Figures 4 and 5 show surface and cross-sectional SEM images of the films deposited using various bias frequencies (10 Hz, 1 kHz, and 100 kHz).The dashed circles in the figures indicate the pores or cracks.The coating was conducted with bias voltage of 0.5 V and the Y 2 O 3 concentration of 0.5 wt% in a suspension solution.For ease of comparison of the SEM images, an SEM image of the film under bias voltage of 0.5 V is shown in Figures 4(b) and 5(b).The mean thicknesses of the films with bias frequencies of 10 Hz, 1 kHz, and 100 kHz were 36.9 m, 25.7 m, and 41.0 m, respectively.The film thickness depended slightly on the bias frequency.For a film deposited with the bias frequency of 10 Hz, many particles were observed on the film surface (Figure 4(a)).Small pores and voids were observed in the film (Figure 5(a)).Furthermore, gas bubbles were generated during film deposition with the bias frequency of 10 Hz because of electrolysis.This electrolysis phenomenon caused some damage (pores and voids) to the resulting film.Both films with bias frequencies of 1 kHz and 100 kHz were dense with pores free from cross-sectional images (Figures 5(b) and 5(c)).A few particles were adsorbed onto the film surface (Figures 4(b) and 4(c)).No great differences between films with bias frequencies of 1 kHz and 100 kHz were observed.A low bias frequency prohibited formation of a dense film, although a high bias frequency (higher than 1 kHz in this investigation) causes formation of a dense film with few adsorptions.
To confirm the effects of bias voltage, Y 2 O 3 films were deposited onto the substrates with different bias voltages.The Y 2 O 3 concentration and the bias frequency were fixed, respectively, as 0.5 wt% and 1 kHz.Figures 6 and 7 present surface and the cross-sectional SEM images of films deposited at various bias voltages: 0.5, 2.0, and 5 V.To compare the SEM images easily, the SEM image of the film under the condition of 0.5 V is depicted again as in Figures 6(a .The greater the bias voltage applied to the substrate at deposition, the more the particles in the suspension solution moved to the substrate electrophoretically.Presumably, the adsorption of large particles at the growing film surface does not cause the formation of a dense film because homogeneous Y 2 O 3 film growth was prevented by the existence of the large particles that had been adsorbed.Furthermore, these adsorptions presumably caused generation of many pores when growing films at higher bias voltages.Thereby, low bias voltage was shown to be suitable for Y 2 O 3 film deposition using a pulsed EPD method. Results showed that Y 2 O 3 dense films were obtainable under the deposition conditions: low Y 2 O 3 concentration (0.5 wt%), high bias frequency (higher than 1 kHz), and low bias voltage (0.5 V).We attempted deposition with a longer deposition time (longer than 1 h), but the film thickness did not correspond to the condition described above.In general, the resistivity of Y 2 O 3 is 10 14 Ω⋅cm [11].When the film thickness was large, the film resistance was high.The effective electrical field of the film surface decreased with increasing film thickness because of the increased film resistance.Advances in Materials Science and Engineering  The present study showed a limitation of Y 2 O 3 film thickness that exists when using the pulsed EPD method with constant bias voltage.
To evaluate the electric insulation of the resulting Y 2 O 3 film, the resistivity was measured for an as-deposited film.Furthermore, the resistivity of a film that was heat-treated at 200 ∘ C and 400 ∘ C was measured.The resistivity of the as-deposited film and the films heat-treated at 200 ∘ C and 400 ∘ C was, respectively, 2.84 × 10 3 Ω⋅cm, 5.36 × 10 4 Ω⋅cm, and 2.05 × 10 6 Ω⋅cm.Although the resistivity of the as-deposited film was lower than the reported value of 1 × 10 14 Ω⋅cm [11], the as-deposited film showed sufficient electrical insulation, which suggests that some limitation of Y 2 O 3 film thickness exists in relation to pulsed EPD method because of the film's high resistivity.The resistivity of the film that had been heat-treated at 200 ∘ C increased corresponding to that of the as-deposited film.This result is assumed to be attributable to residual water removed from films by heat treatment at 200 ∘ C. The resistivity of the film that was heat-treated at 400 ∘ C increased more than that of the film heat-treated at 200 ∘ C, presumably because of the removal of residual citric acid in the films.The resistivity of the film that had been heattreated at 400 ∘ C was 2.05 × 10 6 Ω⋅cm, which was much less than the reported value of 1 × 10 14 Ω⋅cm.The resulting films require some other heat or vacuum treatment to obtain pure Y 2 O 3 films.
A dense Y 2 O 3 film with film thickness of 25.7 m was obtained using pulsed EPD method under deposition conditions of Y 2 O 3 concentration of 0.5 wt%, bias frequency of 1 kHz, bias voltage of 0.5 V, and deposition time of 1 h, but a thicker Y 2 O 3 film is necessary for application to semiconductor production equipment.Therefore, we attempted fabrication of a dense, thick film using two-step deposition with different bias voltages.The first step was deposition with conditions of 0.5 wt% Y 2 O 3 concentration, bias voltage of 0.5 V, bias frequency of 1 kHz, and 1-hour deposition.The second step was increased bias voltage (2.0 V).Other deposition conditions were identical to those of the first deposition.Figure 8 presents SEM images of the films deposited with the second-step bias of 2.0 V.The film thickness produced with the second-step bias of 2.0 V was about 59.8 m.A borderline between the first-step deposition and the second-step deposition was observed at around 30.3 m from the substrate.This result suggests that Y 2 O 3 dense and thick film can be deposited using two-step deposition with changing of the bias voltage.To obtain a dense, thick film using pulsed EPD, two or more deposition steps with different bias voltages are very useful.

Conclusion
Using pulsed EPD, Y 2 O 3 films were deposited.To obtain a dense Y 2 O 3 film using that method, the effective deposition conditions were found to be the following: low Y 2 O 3 concentration solution, high bias frequency, and low bias voltage.Increasing the Y 2 O 3 concentration in a solution slightly decreased the film thickness.The resulting Y 2 O 3 films contain water and some organics derived from the Y 2 O 3 suspension solution.Heat treatment was necessary to remove the residual water and organics from the resulting Y 2 O 3 films.Results show that Y 2 O 3 dense film thickness can be controlled through deposition while changing the bias voltage in two or more steps.

Figure 1 :
Figure 1: TEM image of the precursor Y 2 O 3 nanoparticles.

Figures 2 and 3
present surface and cross-sectional SEM images of films deposited under various Y 2 O 3 concentrations of a suspension solution (0.5, 2.0, and 5.0 wt%).The dashed circles in the figures indicate the pores or cracks.The coating was conducted under bias voltage of 0.5 V and bias frequency of 1 kHz.The mean thicknesses of films with Y 2 O 3 concentrations of 0.5, 2.0, and 5.0 wt% were, respectively, 25.7 m, 23.4 m, and 23.0 m.Increasing the Y 2 O 3 concentration in a solution decreased the film thickness slightly, but the film thickness did not depend much on the Y 2 O 3 concentration in the solution.The film produced using a 0.5 wt% solution was dense with pores that were free from the cross-sectional image (Figure 3(a)).A few particles were adsorbed onto the film surface (Figure 2(a)).Increasing the Y 2 O 3 concentration in the solution increased the adsorbing particles of various sizes including large sizes on the film surface (Figures 2(b) and 2(c)) and an increase in small pores in the films (Figures 3(b) and 3(c)).These large particles were assumed to be the aggregated Y 2 O 3 particles.Aggregation of Y 2 O 3 particles occurred in a high Y 2 O 3 concentration solution.Many large particles were adsorbed onto the growing films' surface at deposition.Presumably, the adsorption of large particles at the growing film surface did not form a dense film because homogeneous Y 2 O 3 film growth was prevented by the existence of the adsorbed large particles.Consequently, dense Y 2 O 3 films with a few adsorptions were obtained using a low Y 2 O 3 concentration solution.

Figure 2 :
Figure 2: Surface SEM images of the films deposited at various Y 2 O 3 concentrations in a suspension solution (0.5, 2.0, and 5.0 wt%), with bias voltage of 0.5 V and bias frequency of 1 kHz.
) and 7(a).The dashed circles in the figures indicate the pores or cracks.The mean thicknesses of the films with bias voltages of 0.5, 2.0, and 5 V were, respectively, 25.7 m, 35.5 m, and 35.1 m.The film thickness increased slightly with increased bias voltage.Increasing the bias voltage caused an increase of particle absorbance onto the film surface (Figures 6(a)-6(c)) and an increase of small pores in the films (Figures 7(a)-7(c))

Figure 3 :
Figure 3: Cross-sectional SEM images of films deposited at various Y 2 O 3 concentrations in a suspension solution (0.5, 2.0, and 5.0 wt%), with bias voltage of 0.5 V and bias frequency of 1 kHz.

Figure 4 :
Figure 4: Surface SEM images of films deposited at various bias frequencies (10 Hz, 1 kHz, and 100 kHz), with bias voltage of 0.5 V and Y 2 O 3 concentration of 0.5 wt% in a suspension solution.

Figure 5 :Figure 6 :
Figure 5: Cross-sectional SEM images of films deposited at various bias frequencies (10 Hz, 1 kHz, and 100 kHz), with bias voltage of 0.5 V and Y 2 O 3 concentration of 0.5 wt% in a suspension solution.

Figure 7 :
Figure 7: Cross-sectional SEM images of films deposited at various bias voltages (0.5, 2.0, and 5 V), with bias frequency of 1 kHz and the Y 2 O 3 concentration of 0.5 wt% in a suspension solution.

Figure 8 :
Figure 8: Cross-sectional SEM images of the films with two-step depositions.The first-step deposition condition was 0.5 wt% Y 2 O 3 concentration, with bias voltage of 0.5 V, bias frequency of 1 kHz, and deposition time of 1 h.The second-step deposition condition was 0.5 wt% Y 2 O 3 concentration, with bias voltage of "2.0 V," bias frequency of 1 kHz, and deposition time of 1 h.